Research Article - Journal of Industrial and Environmental Chemistry (2017) Volume 1, Issue 1
Physicochemical and FTIR studies on Acacia senegal and Anacardium occidentale blendsIdongesit Udo, Stevens A Odoemelam, Nnabuk Okon Eddy*
Department of Chemistry, Michael Okpara University of Agriculture, Umudike, Nigeria
- *Corresponding Author:
- Nnabuk Okon Eddy
Department of Chemistry
Michael Okpara University of Agriculture
E-mail: [email protected]
Accepted Date: October 24, 2017
Citation: Udo I, Odoemelam SA, Eddy NO. Physicochemical and FTIR studies on Acacia senegal and Anacardium occidentale blends. J Ind Environ Chem. 2017;1(1):31-35
Acacia senegal and Anacardium occidentale gums exudate were obtained from a village in Jigawa state, Nigeria. Physicochemical properties were analysed for various blend ratios of Acacia senegal and Anacardium occidentale gums (namely 100:00, 80:20, 60:40, 50:50, 40:60, 20:80 and 00:100). Anacardium occidentale gum is brownish yellow in colour while Acacia senegal gum is white in colour. The two gums absorb maximally at 210 and 200 nm and their conductivity values are 132.40 and 186 µs/cm respectively. Other physical parameters of the gums were salinity (which was similar for the two gums, i.e., 0.1 µs/cm), total dissolved solid (68.40 and 87.80 for Anacardium occidentale and Acacia senegal gum respectively) and turbidity (90 and 27 FAU for Acacia senegal and Anacardium occidentale respectively). Blending at all proportion presented different colours, wavelength of maximum absorption exhibited a gradual reduction at Acacia senegal: Anacardium occidentale blend ratio of 4:1 (205 nm) and gradually stabilizes at 210 nm when the ratio was varied from 1:1 to 2:3 and finally to 1:4. Conductivity was found to decrease from 185.30 to 138.80 µs/cm as the blend ratio of Acacia senegal: Anacardium occidentale changes from 4:1 to 1:4. Similar trend was observed for salinity and total dissolved solid. The FTIR spectra of the blends reveal three set of information. For some blend ratios, the frequency of IR absorption increases with increase in intensity, in others, the frequency and the intensity decreases while in the remaining blends, some functional groups that were present in the parent gums were missing. Therefore, blending significantly alter the physicochemical and FTIR properties of Acacia senegal and Anacardium occidentale gums.
Acacia senegal gums, Anacardium occidentale gums, Blending, Physicochemical and functional properties
Gums are organic substances obtained as an exudation from trunks or branches of the tress naturally or after mechanical injury of the plant by incision of the bark or after the removal of the branch or after invasion by bacteria or fungi [1,2]. They are complex polysaccharides of high molecular weight polymeric compounds [3,4]. Application of gums in most industries cannot be overemphasized. Albizia zygia and some Albizia lebbeck gums are useful as natural emulsifiers in food and pharmaceutical industries [5-7]. Albizia lebbeck gum and gum Arabic are useful in the metallurgical industries . Guar and some other gums have a number of applications in the mining and mineral processing industry . Xanthan and Lucust bean gums are used as thickening agents in food industries . In the froth flotation of base metal and platinum group metal ores, guar gum is used as a depressant of naturally hydrophobic waste minerals such as talc. The role of polysaccharide is to adsorb on the talc surface, render it hydrophilic and prevent its flotation. In the pharmaceutical industries, functional properties of Guar gum are of primary importance for controlling the release of drugs in the gastrointestinal tract, such as carrier for colon targeted drugs, for anti-cancer drugs in the treatment of colorectal cancer and for oral rehydration solutions in the treatment of cholera in adults .
Interestingly, useful applications of gums are based on their function properties including physicochemical, rheological and spectroscopic properties [12-15]. Some may have limited applications and hence limited demand while others may be of great demand but limited supply, indicating that their price could be comparatively high. In order to overcome the problem of scarcity and high demand for some gums (which will ultimately leads to excessive cost), blending is one of the best options of modifying functional properties of gums such that the less demanded and most demanded gums can compete with each other for industrial availability and utilization. The present study is aimed at studying the effect of blending on physicochemical and FTIR spectrum of Acacia senegal (AS) and Anacardium occidentale gum.
Materials and Methods
Crude Acacia senegal (AS), and Anacardium occidentale (AO) gums were obtained as dried exudates from their parent trees grown at Kanya babba village in Bubura local Government Area of Jigawa State (located in North west Nigeria) around mid-November during the day time using the method described by Sharma et al. . The procedure adapted for the purification of the gum was the method reported by Eddy et al. . Composites gums were prepared by combing AO:AS in the following proportions, 80”20, 60:40, 50:50, 40:60, 20:80 respectively. 100% of the respective gums served as the blank.
The moisture content of the gums and their blends were estimated using desicator method as described Dong et al. . In order to estimate the solubility of the gums, analytical balance (Model. XP-3000) was used and the procedures reported by Eddy et al.  was adopted. The pH of the gum was determined using Oaklon pH meter (Model 1100) according to the method reported by Eddy et al. . The Hach colorimeter (Model: DR/890) was used for the determination of the turbidity of the gums and their blends. The wavelengths of maximum absorption for the gums and their blends were determined by scanning the respective samples through various wavelengths using Jenway UV/Vis spectrophotometric (model: 6405) and generating a graph of absorbance against wavelength through which wavelength of maximum absorption, λmax was extrapolated.
FTIR analyses of the gums were carried out out using Scimadzu FTIR-8400S Fourier transform infrared spectrophotometer. The sample was prepared using KBr and the analysis was done by scanning the sample through a wave number range of 400 to 4000 cm-1.
In order to ensure quality data and analysis, recommended analytical methods were adopted for all analysis. Triplicate analysis was also carried out to obtained mean value and ensures reproducibility and reliability of the results obtained. Where necessary, calibration of instrument was carried out.
Physiochemical parameters of Acacia senegal (AS) and Anacardium occidentale (AO) gums are presented in Table 1 while those of the blends are given in Table 2. Frequencies of IR absorption by 100: 0, 80:20, 60: 40, 50:50, 40:60, 20:80 and 0:100 blend of AO and AS by AO gums are recorded in Tables 3 to 9.
Table 1. Physicochemical parameters of Acacia senegal (AS) and Anacardium occidentale (AO) gums.
|Physicochemical parameters||AO gum||AS gum|
|Solubility (water), (Ethanol)||7.7, 0.0||10.8, 0.0|
|pH (@ 27°C)||5.41||5.11|
|Maximum wavelength of absorption (nm)||210||200|
|Total Dissolved Solid (TDS) mg/l||68.4||87.8|
Table 2. Physicochemical parameters of AS:AO gum blends.
|Colour||Peachpuff 1||Bisque||Bisque 2||Navajowhite 2||Wheat|
|Solubility (water),(Ethanol)||9.2, 0.0||8.7, 0.0||8.2, 0.0||7.6, 0.0||7.1, 0.0|
|pH (@ 27°C)||4.53||4.88||4.94||4.81||4.82|
|UV Maximum absorption (nm)||205||215||210||210||210|
|Total Dissolved Solid (TDS) mg/l||94.1||74.5||67.31||70.8||69.81|
Table 3. Frequencies and peaks of IR absorption by AS gum.
|1268||25.89||C-H wag (-CH2X)|
|1424||22.26||C-H in plane bending (CH3)|
|2387||26.35||C=O asymmetric stretching|
|2939||21.7||C-H asymmetric stretch|
Table 4. Frequencies and peaks of IR absorption by AO gum.
|1420||22.89||C-H in plane bending (CH3)|
|3872||32.08||Asymmetric O-H stretching|
Table 5. Frequencies and peaks of IR absorption by 80:20 blend of AO and AS gums.
|2927.08||27.7154||C-H aliphatic stretch|
|3869.33||37.3823||Asymmetric O-H stretching|
Table 6. Frequencies and peaks of IR absorption by 60:40 blend of AO and AS gums.
|878.6||30.53656||=CH out of plane|
|2383.13||38.186||C=O Asymmetric stretching CO2|
|2925.15||22.652||C-H aliphatic stretch|
|3874.16||33.5721||Asymmetric O-H stretching|
Table 7. Frequencies and peaks of IR absorption by 50:50 blend of AO and AS gums.
|877.64||36.862||=CH out of plane|
|2926.11||28.0868||C-H aliphatic stretch|
|3878.98||38.4484||Asymmetric O-H stretching|
Table 8. Frequencies and peaks of IR absorption by 40:60 blend of AO and AS gums.
|878.6||34.7155||=CH out of plane|
|2924.18||26.6011||C-H aliphatic stretch|
|3876.08||42.3019||Asymmetric O-H stretching|
Table 9. Frequencies and peaks of IR absorption by 80:20 blend of AO and AS gums.
|877.64||40.9094||=CH out of plane|
|2924.18||31.9787||C-H aliphatic stretch|
|3862.58||42.3611||Asymmetric O-H stretching|
From Table 1, it is evident that the colour of AS and AO gums are brownish-yellow and white respectively. When the colour of AS and AO gum blend were observed against that of AS as standard gum using the same colour identification method, the blends with 80% AS and 20% AO composition was lighter in shade and the closer in colour when compared to AS gum (Table 2).
Solubility of AO and AS gums in water was 7.7 and 10.8% respectively. The Solubility of the blends of the gum were found to vary with composition. For example, AS:AO ratios of 80:20, 60:40, 50:50, 40:60 and 20:80 displayed solubility values of 9.2, 8.7, 8.2, 7.6 and 7.1% in water respectively. These values are less than the solubility of AS gum (10.8%) indicating that blending tends to lower their solubility with respect to AS gum. However, the solubility of the gum blend increases with increase in the composition of AO gum as shown in Table 2. The pH of AO and AS gums were 5.41 and 5.11 respectively. All the gum blends exhibited pH values that are lower than the pH of the corresponding gums. Generally, for AS:AO blend, the pH increases with increasing ratio.
Measured wavelength of maximum absorbance of AO and AS gums were 210 and 200 nm respectively. Composite mixtures of AS ad AO gum slightly modified the maximum wavelength of absorbance of the gums from 205 to 210 nm for AS:AO ratios of 80:20 and 20:80 respectively. From Beer-Lambert law, absorbance of materials depends on concentration indicating that the composition of the blend is slightly altered. The results obtained clearly reveals that from blend ratio of 50:50, the maximum wavelength of absorbance for AS:AO blend remain steady at 210 nm indicating that after blend ratio of 40:60, the wavelength of maximum absorbance did not depend on the gum composition again. Generally, measurement of maximum wavelength of absorbance has significant analytical implication because it characterized the compound in fixing a reference wave length through which further spectroscopy analysis can be effectively examined on the compound. From the above results, it is evidence that spectroscopy analysis of AO and AS gum blends should be done with due background of their absorbance. The high wavelength of maximum absorption (λmax) noticed in the gum composites may also be attributed to high degree of conjugation which absorb light in the UV or visible regions of the electromagnetic spectrum. Measured turbidity of AO and AS gums were 90 and 27 FAU respectively. Various blends of AS:AO gums presented turbidity values that are relatively comparable to the average turbidity of the crude gums. At blend ratio of 80:20, 60:40, 50:50, 40:60 and 20:80, turbidity values were 54, 120, 122, 128 and 136 FAU. These values increase with increase in the content of AO gum, which had better turbidity than AS gum. Turbidity of AO:KS blends were the highest compared to those measured for other gum blends with similar composition. Generally, the turbidity extends from 352 to 411 FAU and increases with concentration. The present results reveal that blending of gums can significantly altered the turbidity of the composite gums. AO and AS gums have conductivity values of 132.4 and 186μs/cm respectively. AS:AO blends were found to have conductivities of 185.3, 147, 133.8, 139.5 and 138.8 for 80:20, 60:40, 50:50, 40:60, 20:80 composition respectively. Generally, conductivity of the blends tend to decrease with increase in AS content. Total dissolved solid (TDS) is a measure of the combined content of all inorganic and organic substances contained in the gum solution, in a suspended form.
Changes in physicochemical properties of polymer materials due to blending have been reported for several polymers including PCL/PMMA biopolymer , xanthan and locust bean gums , PVC/PMMA [20,21], etc. The results obtained in this study do not conflict with those reported for other polymers.
FTIR is a powerful instrument that can be used to study functional properties of polymer materials and their blend. Several works have been reported on the use of FTIR in studying composites materials derived from polymers. This tool was also employed in this work. As stated before, frequencies of IR absorption by 100: 0, 80:20, 60: 40, 50:50, 40:60, 20:80 and 0:100 blend of AO and AS by AO gums are recorded in Tables 3 to 9.
Functional groups associated with AS gum are C-C bending, CO2, C-O stretch, C-H waging vibration, C-H in plane bending, C=C stretching, C-H stretching vibration, C=O asymmetric stretch, C-H asymmetric stretch, OH stretch and OH stretching. In AS gum, these vibrations occur at frequencies of 25.96, 25.67, 21.83, 25.89, 22.26, 23.06, 26.74, 26.35, 21.70, 13.89 and 20.36 cm-1. In AO gum, C-C bending, CO2 bending, C-O stretching vibration, C-H wagging, C-H in plane , C=G stretch, C-H stretch, OH stretch and OH symmetry stretch were found at 22.94, 22.28, 16.63, 25.81, 22.89, 19.50, 22.27, 11.13 and 32.08 cm-1. It can be seen from the above that the two gums have common functional groups. According to Eddy et al.  gums are polysaccharides and have similar basic constituents, explaining while they have closely related functional groups. The difference between one gum and the other is the frequency and intensity of the IR signal. This indicate that the concentration of the common constituents differ from one gum to another. In AS and AO gums C-C bending was found to occur at 479 cm-1 (intensity=25.96 ) and 476 cm-1 (intensity=22.94).
However, with AO:AS blend ratios of 80:20, 60:40, 50:50 and 40:60, this vibration occurs at a wave number of 416 cm-1 (and intensity of 51.18 ), 419 cm-1 (intensity=40.35), 412 cm-1 (intensity=51.12) and at 421 cm-1 (intensity=38.94) respectively. However, this vibration was absent in the gum composite of composition, 20:80. Therefore blending of AO and AS gum gradually decreases the intensity of C-C bending vibration as the concentration of AO decreases. However, the intensity of the blends are higher than those of 100% AO or AS gum indicating that blending results in modification of the peak of absorption. In AS and AO gums, CO2 vibration occurs at 591 cm-1 (intensity=25.96) and 608 cm-1 (intensity=22.28). However, blending of AO and AS gums at various ratios (80:20, 60:40, 50:50, 40:60, 20:80), the CO2 functional group changed to 587 cm-1 (intensity=30.16 ), 596 cm-1 (22.23), 574 cm-1 (intensity=25.47), 592 cm-1 (23.69) and 556 cm-1 (29.68). Therefore, blending of AO and AS gums produce a composite gum that with shifted frequency and intensity indicating that there is interaction between the two gums . C-O stretching occurs at frequencies of 1057 (intensity=21.83) and 1058 cm-1 (16.63) in AS and AO gums while C-H wagging occurs at 1268 (22.89) and 1258 cm-1 (25.81) respectively. In 80:20 blend of AO and AS gum, the C-O stretch was shifted to 1053 cm-1 (intensity=21.74), the C-H wagging vibration was shifted to 1258 cm-1 (intensity=32.35), C-H bending was shifted to 1412 cm-1 (intensity=29.66), the C=C stretch was shifted to 1634 cm-1 (intensity=29.13), OH stretch was shifted to 3401 (intensity=17.05) and 3869 cm-1 (intensity=37.38). In the 60:40 composite, a new functional group (=CH out of plane) was found at 879 cm-1. C-O stretch was shifted to 1054 cm-1, C-H wagging vibration was shifted to 1263 cm-1, C-H bend was shifted to 1408 cm-1, C=C stretch was shifted to 1634 cm-1, C=O asymmetry appeared at 2383 cm-1, C-H aliphatic stretch was shifted to 2925 cm-1 while OH stretching vibrations were shifted to 3405 and 3874 cm-1 respectively. The =CH out of plane vibration was also found in the spectrum of AO and AS composite containing 50:50 of AO and AS gum. This functional group appeared at 878 cm-1. The C-O stretch, C-H wagging vibration, C-H bending vibration, C=C stretching vibration, and OH vibrations were shifted to 1054, 1263, 1404, 1634, 3408 and 3879 cm-1 respectively. The =CH out of plane signal appear at 592 cm-1 in AO and AS gum composite blended in the ratio, 40: 60. Similarly, C-O vibration, C-H wagging, C=C stretching and OH vibrations were shifted to 1054, 1266, 1406, 1632, 3393 and 3876 respectively. At 878 cm-1, the =CH out of plane vibration was also found in the spectrum of AO/AS composite whose composition was 20: 80 (i.e., AO:AS ratio). CO stretch was shifted to 1055 cm-1, C-H wagging vibration was shifted to 1277 cm-1, C-H bending to 1402 cm-1, C=C vibration to 1635 cm-1 and OH vibrations were shifted to 3385, 3447 and 3862 cm-1. It is evident that there are forward and backward shifts in some functional groups due to blending. Few new functional groups that were not common to AO or AS were also formed. The intensities of the respective functional groups were also observed to change significantly. Therefore, during blending, there is interaction and the composite may possess properties or assumed a new form. The shift in FTIR frequency due to bleding obtained in this work agrees with the results obtained from others with respect to polymer-polymer blends [16,18,19].
This study was designed to investigate the effect of blending on the physicochemical and functional properties of AO and AS gums. From the results and findings of the study, it can be concluded that blending has significant effect on the physicochemical properties of the gums. The functional properties of the gums composites are found to be shifted in frequency and intensity of infra-red absorption as a result of blending. Therefore, functional properties of gums can be modified for broader applications through blending.
- Ahmed SE, Babiker EM, Ahmed KK. Analytical studies on the gum exudates from Anogeissus leiocarpus. Pak J Nutr. 2009;8(6):782-6.
- Bhushete PR, Annapure US. Comparative study of Acacia nilotica exudate gum and Acacia gum. Intern. J Biol Macromol. 2007;102:266-71.
- Ameh, P, Eddy NO, Gimba CE. Physiochemical and rheological studies on some natural polymers and their potentials as corrosion inhibitors. Lambert Academic Publishing, UK. 2012.
- Eddy NO, Udofia I, Uzairu A. Physicochemical, spectroscopic and rheological characterization of Albizia lebecck gum exudates. Pigment and Resin Technol. 2014;43(4):228-44.
- Anderson DMW, McDougall FJ. Degradative studies of gum arabic (Acacia senegal (L.) Willd) with special reference to the fate of the amino acids present. Food Additives and Contaminants. 1987;4(3):247-55.
- Anderson DMW, Wang WP. The tree exudates permitted in foodstuffs as emulsifiers, stabilizers and thickeners. Chem Ind Forest Prod. 1994;14(2):73-83.
- Mhinzi GS. Chemotaxonomic distinction of selected closely related acacia species using chemical properties of their gum exudates. Tanz J Sci. 2003;29(1):91-8.
- De Paula RCM, Santana SA, Rodrigues JF. Composition and rheological properties of Albizia lebbeck gum exudates. Carb Poly. 2001;44:133-9.
- Ma X, Marek P. Intrinsic viscosities and huggins constants of guar gum in alkali metal chloride solutions. Carb Poly A. 2007;70:15–24.
- Higiro J, Herald TJ, Alavi S. Rheological study of xanthan and locust bean gum interaction in dilute solution. Food Res Intern. 2006;39:165–175.
- Pablyana LRC, de paula CMR, Feitosa PA. Purification of guar gum for biological applications. Int J Biol Macromol. 2007;41:324-31.
- Eddy NO, Udofia I, Abechi SE, et al. Rheological modeling, spectroscopic and physicochemical characterization of Raphiahookeri gum exudates. Walialak J Sci Technol. 2015;12(5):407-29.
- Fadavi G, Mohammadifar MA, Zargarran A, et al. Composition and physicochemical properties of Zedo gum exudates from Amygdalus scoparia. Carb Poly A. 2014;101:1074-1080.
- Shi Y, Li C, Zhang L, et al. Characterization and emulsifying properties of octenyl succinate anhydride modified Acacia seyal gum (gum Arabic). Food hydrocolloids. 2017;65:10- 16.
- Mehrnia M, Jafari S, Makhmal-Zadeh, et al. Rheological and release properties of double nano-emulsions containing crocin prepared with Angum gum, Arabic gum and whey protein. Food Hydrocoll. 2017;66:259-67.
- Sharma VK, Maxumder B, Nautiyah V. Rheological characterization of Isabgol husk, gum katira hydrocolloids and their blends. Int J Food Sci. 2014.
- Dong Y, Sørensen KM, He S, et al. Gum arabic authentication and mixture quantification by near infrared spectroscopy . Food Contr. 2017;78:144-9
- Abdelrazek EM, Hezma AM, El-khodary A, et al. Spectroscopic studies and thermal properties of PCL/PMMA biopolymer blend. Egyptian J Basic Appl Sci. 2006;3:10-15.
- Higiro J, Herald TJ, Alavi S, et al. Rheological study of xanthan and locust bean gum interaction in dilute solution: Effect of salt. Food Res Intern. 2007;40:435-47.
- Ramesh S, Leen KH, Kumutha K, et al. FTIR studies of PVC/PMMA blend based polymer electrolytes. Spectrochimica Acta Part A. 2007;66:1237-42.
- Rajendran S, Uma T. Conductivity on PVC/PMMA polymer blend electrolyte. Mat Let. 2000;44:242-7.